Gelatin Properties of Goat Skin Produced by Calcium Hydroxide as Curing Material
M. I. Saida,*, S. Triatmojob, Y. Erwantob, & A. Fudholic aFaculty of Animal Science, Hasanuddin University Jln. Perintis Kemerdekaan Km.10, Makassar 90245 Indonesia
bFaculty of Animal Science, Gadjah Mada University Jln. Fauna 3 Bulaksumur, Yogyakarta 55281 Indonesia
cFaculty of Pharmacy, Gadjah Mada University Sekip Utara, Yogyakarta 55281 Indonesia (Received 14-12-2010; accepted 25-08-2011)
Penerapan basa kuat sebagai bahancuring telah banyak diterapkan dalam industri gelatin komer-sial, namun penerapan basa lemah belum banyak dilakukan. Penerapan basa kuat sebagai bahan curing tidak ekonomis dan diduga dapat berpengaruh bagi kesehatan manusia. Penelitian dilakukan untuk mempelajari sifat-sifat gelatin kulit kambing yang diproduksi menggunakan basa lemah jenis Ca(OH)2 dan selanjutnya dibandingkan dengan sifat-sifat gelatin komersial. Kulit kambing dari jenis Bligon (hasil persilangan kambing etawah dan kacang) jantan umur 1,5-2,5 tahun digunakan sebagai bahan baku dan Ca(OH)2100 g/l sebagai bahan curing. Rancangan acak lengkap pola faktorial 2x3 dengan 3 ulangan digunakan sebagai desain penelitian. Dua waktucuring (2 dan 4 hari) dan tiga kon-sentrasi bahan (3, 6, 9% v/v) digunakan sebagai perlakuan serta gelatin komersial (murni oleh Merck, standar pangan dan standar farmasi) digunakan sebagai kontrol. Gelatin yang diproduksi dari kulit kambing menggunakan Ca(OH)2 memiliki sifat yang mirip dengan gelatin komersial. Kadar logam berat (Pb, Cu, dan Zn) yang dikandung dalam produk gelatin kulit kambing masih memenuhi standar yang dipersyaratkan SNI. Produksi gelatin optimum dihasilkan dari penerapan waktu curing 4 hari pada konsentrasi 9% (v/v).
Kata kunci: kulit kambing, bahan curing, basa lemah, sifat gelatin
Application of strong bases as curing materials has been widely applied in commercial gelatin industries, but the application of weak bases has not been much done. Application of strong bases as a treatment was not economical and assumed to aﬀ ect human health. Studies were conducted on the properties of goat skin gelatin manufactured using weak base types of Ca(OH)2and then compared with properties of commercial gelatin. Skins from Bligon goats of 1.5 to 2.5 years old was used as the raw materials and Ca(OH)2 100 g/l as curing materials. The 2x3 factorial completely randomized design (CRD) with three replications was used as a design study. Two curing times (2 and 4 days) and three concentrations (3, 6, 9% v/v) were used as treatments, and commercial gelatin (pure (P) by Merck, food grade (Fg) and pharmacy standards (Ps)) were used as control. Gelatin produced from goat skins using Ca(OH)2 had properties similar to that of commercial gelatin. The heavy metals (Pb, Cu and Zn) contained in goat skin gelatin still meet the INS standards. The optimum production of gelatin has been generated through the application of 4-day curing time at a concentration of 9% (v/v).
Key words: goat skin, curing materials, weak base, gelatin properties
* Corresponding author: e-mail: firstname.lastname@example.org
Accredited by DGHE No: 66b/DIKTI/Kep/2011 DOI: 10.5398/medpet.2011.34.3.184
The amount of commercial gelatin as a raw material of food and pharmaceutical industries in the country is
In the process of gelatin production required a cur-ing step to improve the quality of gelatin (Kolodziejska et al., 2003). Curing materials from the group of acids and bases (strong or weak) have been widely applied in gelatin production process from raw materials, par-ticularly the skin and bones of ﬁ sh (Gudmundsson, 2002; Jamilah & Harvinder, 2002; Kolodziejska et al., 2003; et al., 2005; Kasankala et al., 2007)
the application of curing material from the skin of a goat have not been published. So far, the use of strong acid (i.e.HCl) and strong base (i.e. NaOH) as curing materials of commercial gelatin production process is expensive and it is assumed to aﬀ ect human health.
The use of curing materials of weak base (ie. Ca(OH)2) has not been widely applied, especially in the production process of gelatin made from raw goat skins. Ca(OH)2 is more economical as well as relatively safe for human health and easier to obtain. The application of the curing time and the concentration of Ca(OH)2 with the right combination are required in the production of
process. The use of curing materials with incorrect com-bination can be aﬀ ected by the quality of gelatin (Wang et al., 2008b; Zeugoliset al., 2008). In this case, the study was conducted to determine the properties of gelatin made from goat skins manufactured using materials curing Ca(OH)2 and to determine the optimal treatment combination.
MATERIALS AND METHODS
A total of 10 pieces of goat skin from Bligon male, 1.5 to 2.5 years old were used as a raw material. Bligon
Calcium hydroxide (Ca(OH)2 100 g/l) was used as a cur-ing material.
Preparation of raw materials. Raw skin was weighed and washed in running water for 30 min. Raw skin was soaked in a solution of 1% teepol and washed in running water for 15 min. Fleshing machine was used to remove the remaining ﬂ esh and fat. Solution of 2% lime + 3% Na2S was used in unhairing process. The skin was washed with running water for 15 min and continued with the process of neutralization in a solution of 2% HCOOH (pH 7-7-5). Sheets of skin without hair were cut into small pieces the size of 3x3 cm. The skin pieces were combined into a single (composite) for use as raw material of gelatin.
Preparation of curing solution. Calcium hydroxide (Ca(OH)2 100 g/l) concentrations of 3%, 6%, and 9% (v/v) were used as treatments. Curing solution concentration of 3%, 6%, and 9% was made by dissolving Ca(OH)2 100 g/l each of 3, 6 and 9 ml into a ﬂ ask containing 100 ml of distilled water to limit the volume of 100 ml.
Preparation of materials. Gelatin was produced in ac-cordance with Ockerman & Hansen (2000) methods. The composite raw material soaked in a curing solution at 5-10 °C temperature. The curing time and concentra-tion of the soluconcentra-tion was used to adapt to treatment. Raw materials were neutralized with acetic acid to pH 6 to 7.5, weighed and extracted. The extraction process was performed on three steps: step I (55-60oC); step II (60-65 oC), and step III (65-70 °C) each for 3 hours. The extract
was ﬁ ltered and concentrated at 70 °C for 2 hours. It was cooled in a refrigerator at 5-10oC for 30 min and dried at 55 °C for 18-20 hours until the gelatin sheet solid. The gelatin sheets were milled and packaged in vacuum plas-tic to test its properties.
Method of Analysis
Gel strength (Muyongaet al., 2004 ; Liuet al., 2008) (Mod-iﬁ cation). Gel strength was measured with a Universal Testing Machine (Zwick/Z 0.5). Gelatin solution 6.67% w/ v (6.67 grams to 100 ml distilled water) was heated at the temperature of ± 60°C to dissolve the particles. Solution in the container Ø 5 cm and a height of 6 cm was stored at 5o
of the plunger (Ø= 13 mm). The test was conducted at the temperature of ±10 °C and the speed 10 mm/min as deep as 4 mm was used as plunger. The value of gel strength (g Bloom) used the formula= 20 + 2.86.10-3 D, where D= F/G x 980, F= height chart before fracture; G= constant (0.07).
Protein content (AOAC, 2005). FOSSKjeltec 2200 was used to determine protein content. A total of 0.5 g of sam-ple + ¼bussino tablet + 12 ml of H2SO4 was concentrated in the destruction of the tube FOSS at ± 410oC for 1 hour. The results of destruction was distilled with thio-NaOH 40% + H3BO4 4% + BCGMR indicators. A total of 150 ml was destilated in erlemenyer disk and titrated with 0.099 N HCl until the color changed from blue to pink. Five point ﬁ fty ﬁ ve (5.55) was used as the conversion factor of gelatin protein. The protein content (%) was calculat-ed using the formula= ((ml HCl – ml Blanko) x N HCl x 14,008 x 100 x 5,55)/g sample x 1000.
Fat content (AOAC, 2005). A total of 2 g sample + petro-leum ether was incorporated into theSoxhlet ﬂ ask which was dried at 105oC for 2 hours. Water bath for ± 3 hours was used to reﬂ ux process, dried in the oven for 1 hour ± 105oC, and cooled in a desiccator. The fat content (%) was calculated using the formula= (fat weight (g)/sample weight (g)) x100%.
Water activity (aw) (Sudarmadji et al., 2007). awmeter (Decagon Divice Pullman WA 99163, USA) was used to determine the aw value. A total of 3 g sample was placed
wmeter, left for 3 min, and the result could be read on the monitor.
aquadest was added to the rest and warmed for several minutes. The results were ﬁ ltered and washed until 100 ml ﬁ ltrate was obtained. A total of 8 ml of ﬁ ltrate was diluted with aquadest until the reach volume 25 ml and the value of heavy metals was determined.
Organoleptic characteristics (Soekarto, 2008). Goat skin gelatin products and commercial were packaged with plastic clips and then photographed with a digital ca-mera (Olympus FE-20).
Experimental Design and Data Analysis
A 2x3 completely randomized design (CRD) factor with three replications was used as the experimental design. Factor I, two curing time (2 and 4 days), and factor II, three concentrations of curing materials (3, 6 and 9% v/v), each was repeated 3 times. Data results of an experiment (gel strength, protein content, fat content and aw value) were analyzed by ANOVA, while the data content of heavy metals and organoleptic characteristics of gelatin were analyzed descriptively. The treatment showing a signiﬁ cant eﬀ ect was tested its diﬀ erence by Duncan Multiple Range Test (DMRT) at 5% level.
RESULTS AND DISCUSSION
Gel strength of gelatin is very important on physical properties. Gel strength is aﬀ ected by hydrogen bonds between water molecules and free hydroxyl groups of amino acid groups, the size of the protein chain, con-centration, and molecular weight distribution of gelatin (Bhat & Karim, 2009). The comparison between gel strength of gelatin produced from goat skin and com-mercial gelatin was presented in Figure 1.
The increasing use of Ca(OH)2 concentration tends increased the value of gel strength (Figure 1). Gel strength of goat skin gelatin produced in the range of 75.77 to 97.81 gBloom is lower than that of commercial
gelatin. The highest gel strength of the production process used concentration of 9% Ca(OH)2with a curing time of 4 days. Gel strength of gelatin was aﬀ ected by concentration of curing materials. Application of high concentrations of curing materials in gelatin produc-tion process tends to increase the gel strength values (Ockerman & Hansen, 2000). Gel strength was aﬀ ected by the concentration of materials and curing time, it is one parameter to determine the physical quality of a product on gelatin (Kolodziejska et al., 2003). The con-centration, curing times, and temperature had signiﬁ cant eﬀ ect on the amount of collagen which dissolved during the extraction process (Wanget al., 2008b). The concentra-tion is one important variable that can aﬀ ect the ability to extract collagen (Zhanget al., 2007).
The application of diﬀ erent concentration and curing time and their interaction had signiﬁ cant eﬀ ect (P<0.01) on the gel strength. Gel strength properties were associated with hydrogen bonds between water molecules and free hydroxyl groups of amino acid groups, the size of the protein chain, concentration, and molecular weight distribution of collagen (Arnesen & Gildberg, 2002; Bhat & Karim, 2009). In general, gel strength of gelatin was produced close to the results obtained by previous researcher that was 75-275 gBloom (Ockerman & Hansen, 2000).
Gelatin is the collagen protein, a group derived from the structural proteins and extracellular matrix and produced in large quantities (Karim & Bhat, 2008). The diﬀ erence in curing time and concentration of Ca(OH)2 and their interaction had no signiﬁ cant eﬀ ect on protein content of gelatin (Table 1). This may be caused by dif-ferences in the rate applied. According to Wang et al. (2008a), the decreasing of amino acids concentrations led to some bonds that form the collagen protein to break down. Furthermore, Muyonga et al. (2003) explained that the curing material could damage the structure of the amino acids on the denaturation process.
Protein content from goat skin gelatin was not diﬀ erent from commercial gelatin (Table 4). Songchotikunpan et al. (2007) said that 89.4% protein content of gelatin was produced from Red Tilapia ﬁ sh (Oreochromis niloticus) and 80.9%-86.6% from sword ﬁ sh (Astawan & Aviana, 2003).
The application of curing time and concentration of Ca(OH)2 and their interaction had no signiﬁ cant eﬀ ect on the fat content (Table 2). This might be caused by the use of the same extraction temperature in the produc-tion process. In the skin, there was a great amount of fat that was bound to proteins (lipoproteins). At the time of the extraction process with the same temperature, the protein would be broken, followed by the release of
et al. (2008) and Wanget al. (2008b), during the
extrac-microbial growth. Sudarmadji et al. (2007) illustrated that aw value usually increased when a food product absorbed air from the environment as a result of the storage time process. Food products were located in the open air and the water level would reach equilibrium with the ambient humidity.
Heavy Metals Content (Pb, Cu, and Zn)
One of the food safety requirements on the product gelatin was that heavy metals content must not exceed the allowed limit. Comparison of heavy metals content (Pb, Cu and Zn) in the goat skin gelatin, commercial gelatin (control), and Indonesian National Standards (INS) was presented in Figure 2.
The values of Pb metal in the goat skin gelatin and commercial vary (Figure 2a). The amount of Pb metal found in the treatment of T2C3, T2C9, T4C3, and T4C9 was higher than other treatments and control, but still lower than the requirements of INS (50 ppm) (INS, 2005). Figure 2b showed that Cu metal were higher in the treat-ment of T2C3, T2C6, T4C3 and T4C6 than others, but lower than the commercial, especially food grade gelatin (Fg) and than INS standard (30 ppm) (INS, 2005), while Figure 2c showed that goat skin gelatin and commercial contained Zn metal with diﬀ erent values, but lower than standard INS (100 ppm) (INS, 2005). Particularly in the commercial gelatin (food grade), the Zn metal was the highest.
Heavy metal elements contained by the goat skin gelatin were likely to come from: (1) feed and drinking water consumed by the goats and stored in the skin tis-sue, (2) water from the skin processing (soaking, unhair-ing, washing and neutralization), and (3) contamination of equipment in the production process.
Table 1. Protein content (%) of gelatin from goat skin in some conditions
Curing time (days)
Concentration of Ca(OH)2 (%) (v/v)
3 6 9
2 92.05±0.89 92.03±1.63 93.60±2.37
4 91.63±2.53 93.01±1.25 92.45±2.03
Table 3. Water activity (aw) value of gelatin from goat skin in some conditions
Table 4. Chemical composition of commercial gelatin products as control
Curing time (days)
Concentration of Ca(OH)2 (%) (v/v)
3 6 9
Table 2. Fat content (%) of gelatin from goat skin in some condi-tions
Curing time (days)
Concentration of Ca(OH)2 (%) (v/v)
3 6 9
2 0.45±0.23 0.55±0.29 0.43±0.19
4 0.45±0.19 0.48±0.25 0.43±0.19
tion process, it will cleavage structures of protein until it ﬁ nally dissolves.
The fat content of goat skin gelatin and that of com-mercial gelatin did not diﬀ er much (Table 4). The previ-ous results also showed that the fat content 0.3% from Red Tilapia ﬁ sh (Oreochromis niloticus) (Songchotikunpan et al., 2007) and 0.47% to 1.7% from sword ﬁ sh (Astawan & Aviana, 2003) was same with commercial gelatin.
Water Activity (aw) Value
Figure 3. Physical appearance of the gelatin; (a) goat skin gelatin produced by (Ca(OH)2; (b) pure (P) by Merck; (c) food grade (Fg), and (d) pharmacy standart (Ps).
Organoleptic properties were important to consider because it related to consumer considerations in choos-ing a product (Suryati et al., 2006). Organoleptic refers to any sensory properties of a product, involving taste, colour, odour and feel. Organoleptic testing involves inspection through visual examination, feeling and smelling of products. According to Soekarto (2008), the organoleptic tests had high relevance to the quality of the product because it deals directly with consumer tastes. The comparison of organoleptic characteristics of goat skin gelatin and commercial was presented in Figure 3.
Figure 3 showed goat skin gelatin produced by alkali processes with Ca(OH)2 had a color similar to the commercial gelatin, a yellowish color as standard (INS, 2005). In addition to color, goat skin gelatin was more
smooth and uniform than the food grade gelatin (Fg). According to Tyler & Gregory (2005), the color diﬀ er-ences on food products can be caused by the eﬀ ect of temperature and pH in the production process.
The gelatin of goat skin produced using weak base (CaOH)2 had similar gel strength, protein content, fat content, aw value, and color to the commercial gelatin. Optimum production results have been obtained from a combination of curing time of 4 days with a concentra-tion of 9% (v/v).
Thanks to the Directorate-General of Higher Education, Ministry of National Education of Indonesia for the ﬁ nancial support through the research grants program for PhD students.
AOAC. 2005. Oﬃ cial Methods of Analysis of AOAC Interna-tional. 18th ed. Assoc. Oﬀ . Anal. Chem., Arlington.
Arnesen, J. A. & A. Gildberg. 2002. Preparation and character-ization of gelatine from the skin of harp seal (Phoca groend-landica). Bioresource Technology. 82: 191-194.
Astawan, M. & T. Aviana. 2003. The inﬂ uence of type solution and drying methods on the physical properties, chemical and functional gelatin of skin from sword ﬁ sh. J. Tech. & Food Indust. 14: 7-13.
Bhat, R. & A. A. Karim. 2009. Ultraviolet irradiation improves gel strength of ﬁ sh gelatin. Food Chem. 113: 1160-1164 doi:10.1016/j.foodchem.2008.08.039.
Chiou, B., R. J. Avena-Bustillos, P. J. Bechtel, H. Jafri, R. Na-rayan, S. H. Imam, G. M. Glenn, & W. J. Orts. 2008. Cold water ﬁ sh gelatin ﬁ lms: Eﬀ ects of cross-linking on ther-mal, mechanical, barrier, and biodegradation properties. European Polymer Journal 44: 3748-3753. doi:10.1016/ j.eurpolymj.2008.08.011.
Duan, R., J. Zhang, X. Du, X. Yao, & K. Konno. 2008. Proper-Figure 2. Comparison of heavy metals content of goat skin
gelatin with commercial and INS; (a) Pb; (b) Cu; (c) Zn; T2= curing time of 2 days; T4= curing time of 4 days; C3= concentration of 3%; C6= concentration of 6%; C9= concentration of 9%; P= pure by merck; Fg= food grade; Ps= pharmacy standart; INS= Indonesian National Standards. Means with diﬀ erent superscript diﬀ er signiﬁ cantly (P<0.05).
ties of collagen from skin, scale and bone of carp (Cyprinus carpio). Food Chem. 112: 702-706.
Gilsenan, R. M., P. M. Gilsenan, & S. B. Ross-Murphy. 2000. Rheological characterisation of gelatins from mammalian and marine sources. Food Hydrocolloid 14: 191–195.
Giménez, B., M. C. Gómez-Guillén, & P. Montero. 2005. The role of salt washing of ﬁ sh skins in chemical and rheologi-cal properties of gelatin extracted. Food Hydrocolloids. 19: 951-957.
Gómez-Estaca, J., L. Bravo, M. C. Gómez-Guillén, A. Alemán, & P. Montero. 2008. Antioxidant properties of tuna-skin and bovine-hide gelatin ﬁ lms induced by the addition of oregano and rosemary extracts. Food Chem. 112: 18-25.
Gómez-Guillén., M. C., J. Turnay, M. D. Fernández-Dı´az, N. Ulmo, M. A. Lizarbe & P. Montero. 2002. Structural and physical properties of gelatin extracted from diﬀ erent ma-rine species: A comparative study. Food Hydrocolloids 16: 25–34.
Grobben, A. H., P. J. Steele, R. A. Somerville, & D. M. Taylor.
2004. Inactivation of the bovine-spongiform-encephalopathy (BSE) agent by the acid and alkali processes used in the manufacture of bone gelatine. Biotech and App. Biochem. 39: 329-338.
Gudmundsson, M. 2002. Rheological properties of ﬁ sh gelatin. J. Food Sci. 67: 2172-2175.
Hambidge, K. M. & N. F. Krebs. 2007. Zinc deﬁ ciency: a spe-cial challenge. J. Nut.: 137 (Abstr.).
Hidaka, S. & S. Y. Liu. 2002. Eﬀ ect of gelatins on calcium phos-phate precipitation: a possible application for distinguish-ing bovine bone gelatin from porcine skin gelatin. J. Food Comp. Analy. 16: 477-483.
INS.2005. Indonesian National Standards. Number 06-3735-1995 about gelatin products. National Standardization Agency. Ministry of Industry and Trade of the Republic of Indonesia, Jakarta.
Jamilah, B & K. G. Harvinder. 2002. Properties of gelatins from skins of ﬁ sh black tilapia (Oreochromis mosambicus) and red tilapia (Oreochromis nilotica). Food Chem. 77: 81-84.
Jongjareonrak, A., S. Benjakul, W. Visessanguan, & M. Tana-ka. 2008. Antioxidative activity and properties of ﬁ sh skin gelatin ﬁ lms incorporated with BHT and α-tocopherol. Food Hydro. 22: 449-458.
Karim, A. A. & R. Bhat. 2008. Gelatin alternatives for the food industry: recent developments, challenges and prospects. Trends in Food Sci. & Tech. 19: 644-656. doi:10.1016/ j.tifs.2008.08.001 (In Press).
Kasankala, L. M., Y. Xue, Y. Weilong, S. D. Hong, & Q. He.
2007. Optimization of gelatine extraction from grass carp (Catenopharyngodon idella) ﬁ sh skin by response surface methodology. Bioresource Tech. 98: 3338-3343.
S. Benjakul, W. Visessanguan, T. Na-gai & M. Tanaka. 2005. Characterisation of acid-soluble collagen from skin and bone of bigeye snapper (Priacan-thus tayenus). Food Chem. 89: 363–372.
Kolodziejska, I., K. Kaczorowski, B. Piotrowska, & M. Sad-owska. 2003. Modiﬁ cation of the properties of gelatin from skins of Baltic cod (Gadus morhua) with transglutaminase. Food Chem. 86: 203-209.
Liu, H. Y., J. Han & S. D. Guo. 2008. Characteristics of the gela-tin extracted from channel catﬁ sh (Ictalurus punctatus) head bones. Food Sci. and Tech. 43: 313-317.
Muyonga, J. H., C. G. B. Cole & K. G. Duodu. 2004. Extraction and physico-chemical characterization of Nile perch (Lates niloticus) skin and bone gelatin. Food Hydrocolloids.18:
Muyonga, J. H., C. G. B. Cole & K. G. Duodu. 2003. Fourier transform infrared (FTIR) spectroscopic study of acid sol-uble collagen and gelatin from skins and bones of young and adult Nile perch (Lates niloticus). Food Chem. 86: 325-332.
Ockerman, H. W. & C. L. Hansen. 2000. Animal by Product Processing and Utilization. CRC Press, USA.
Soekarto, S.T.2008. Organoleptic Assessment for the Food In-dustry. Bogor Institute of Agriculture, Bogor.
Songchotikunpan, P., 2007.
Ex-traction and electrospinning of gelatin from ﬁ sh skin. Internl. J. Biol. Macromolec. 42: 247-255.
Sudarmadji, S., B. Haryono, & Suhardi. 2007. Analysis of Food and Agriculture. Issue 2nd. Cooperation Liberty of Yogya-karta with the Inter-University Centre for Food and Nutri-tion, Gadjah Mada University, Yogyakarta.
Suryati, T., M. Astawan, & T. Wresdiyati. 2006. Characteristics organic of meat sheep given a low voltage electrical stimu-lation and injection of calcium chloride. Med.Pet. 29: 1-6.
Tyler, J. H. & R. D. Gregory. 2005. An expeditions, high yield construction of the food aroma compound 6-acetyl-1,2,3,4-tetrahydropyridine and 2-4 acetyl –1pyrrolyne. Journ. org. chem. 70: 10872–10874.
Wang, L., M. A. E. Auty, A. Rau, J. F. Kerry, & J. P. Kerry. 2008a. Eﬀ ect of pH and addition of corn oil on the properties of gelatin based biopolymer ﬁ lm. J. Food Eng. 90: 11-19.
Wang, L., B. Yang, R. Wang, & X. Du. 2008b. Extraction of pep-sin-soluble collagen from grass carp (Ctenopharyngodon idella) skin using an artiﬁ cial neural network. Food Chem. 111: 683-686.
Yudhabuntara, D. 2008. Control of Microorganisms in Food.
ganisms -in-food.html [December 23, 2009].
Zeugolis, D. I., S. T. Khew, E. S. Y. Yew, A. K. Ekaputra, Y. W. Tong, L. L.Yung, D. W. Hutmacher, C. Sheppard, & Mi-chael. 2008. Electro-spinning of pure collagen nano-ﬁ bres – Just an expensive way to make gelatin ?. Biomaterials. 15: 2293-2305.